#------------------------------------------------------------------------------
#$Date: 2016-03-26 21:32:27 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180477 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/46/7214667.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7214667
loop_
_publ_author_name
'Wang, Xiuli'
'Xu, Chuang'
'Lin, Hongyan'
'Liu, Guocheng'
'Yang, Song'
'Gao, Qiang'
'Tian, Aixiang'
_publ_section_title
;
 Tuning the architectures of polyoxometalate-templated complexes by
 changing the spacer lengths of bis-pyridyl-bis-amide ligands (L): from 1D
 chains to 2D networks based on different (CuL)n loops
;
_journal_issue                   18
_journal_name_full               CrystEngComm
_journal_page_first              5836
_journal_paper_doi               10.1039/c2ce25371b
_journal_volume                  14
_journal_year                    2012
_chemical_formula_sum            'C54 H86 Cu2 Mo12 N12 O56 Si'
_chemical_formula_weight         3105.80
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                100.6390(10)
_cell_angle_beta                 108.6950(10)
_cell_angle_gamma                91.2210(10)
_cell_formula_units_Z            1
_cell_length_a                   11.3637(9)
_cell_length_b                   12.9558(11)
_cell_length_c                   16.8671(14)
_cell_measurement_temperature    293(2)
_cell_volume                     2303.2(3)
_computing_structure_refinement  'SHELXS-97 (Sheldrick, 2008)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.995
_diffrn_measured_fraction_theta_max 0.995
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0199
_diffrn_reflns_av_sigmaI/netI    0.0185
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       21
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            36562
_diffrn_reflns_theta_full        27.00
_diffrn_reflns_theta_max         27.00
_diffrn_reflns_theta_min         1.30
_exptl_absorpt_coefficient_mu    2.145
_exptl_absorpt_correction_T_max  0.7253
_exptl_absorpt_correction_T_min  0.6860
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            green
_exptl_crystal_density_diffrn    2.239
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             1518
_exptl_crystal_size_max          0.19
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_refine_diff_density_max         1.546
_refine_diff_density_min         -1.647
_refine_diff_density_rms         0.174
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.097
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     681
_refine_ls_number_reflns         10012
_refine_ls_number_restraints     3
_refine_ls_restrained_S_all      1.101
_refine_ls_R_factor_all          0.0431
_refine_ls_R_factor_gt           0.0396
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0408P)²+10.6913P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1024
_refine_ls_wR_factor_ref         0.1047
_reflns_number_gt                9307
_reflns_number_total             10012
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2ce25371b.txt
_cod_data_source_block           4
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_database_code               7214667
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Cu1 Cu 0.0000 0.0000 0.5000 0.0400(2) Uani 1 2 d S . .
Cu2 Cu -1.4882(3) 0.52247(14) 0.0046(2) 0.0504(5) Uani 0.50 1 d P . .
Si1 Si 0.0000 0.0000 0.0000 0.0220(3) Uani 1 2 d S . .
Mo1 Mo 0.02367(4) 0.08306(3) 0.21559(2) 0.02958(9) Uani 1 1 d . . .
Mo2 Mo 0.00109(4) -0.18980(3) 0.12528(2) 0.03328(10) Uani 1 1 d . . .
Mo3 Mo -0.03117(4) 0.26724(3) 0.07888(3) 0.03781(11) Uani 1 1 d U . .
Mo4 Mo 0.27971(4) -0.11457(4) 0.09114(3) 0.04123(12) Uani 1 1 d U . .
Mo5 Mo 0.26021(4) 0.04001(3) -0.06457(3) 0.03024(9) Uani 1 1 d . . .
Mo6 Mo 0.26200(4) 0.16144(3) 0.14131(3) 0.03687(11) Uani 1 1 d U . .
O1 O -0.0439(5) -0.0242(4) 0.0746(3) 0.0216(11) Uani 0.50 1 d P . .
O2 O 0.0486(5) 0.0922(4) 0.0855(3) 0.0209(11) Uani 0.50 1 d P A .
O3 O 0.1524(5) 0.0214(4) 0.0298(3) 0.0213(11) Uani 0.50 1 d P . .
O4 O 0.0579(5) -0.1119(4) 0.0283(3) 0.0195(10) Uani 0.50 1 d P . .
O5 O 0.0357(10) -0.0570(8) 0.2286(6) 0.0308(13) Uani 0.525(11) 1 d P A 1
O5' O 0.0509(11) -0.0518(9) 0.2014(7) 0.0308(13) Uani 0.475(11) 1 d P A 2
O6 O 0.1903(6) 0.1409(5) 0.2434(4) 0.0316(10) Uani 0.509(7) 1 d P A 1
O6' O 0.1662(7) 0.1072(6) 0.2010(5) 0.0316(10) Uani 0.491(7) 1 d P A 2
O7 O 0.3519(7) 0.0245(6) 0.1599(4) 0.0320(10) Uani 0.496(7) 1 d P A 1
O7' O 0.2858(7) 0.0094(5) 0.1494(4) 0.0320(10) Uani 0.504(7) 1 d P A 2
O8 O 0.1937(6) -0.1883(6) 0.1541(4) 0.0356(9) Uani 0.503(6) 1 d PU A 1
O8' O 0.1702(6) -0.1369(6) 0.1357(4) 0.0356(9) Uani 0.497(6) 1 d P A 2
O9 O -0.0249(6) 0.2283(5) 0.1901(5) 0.0296(10) Uani 0.506(7) 1 d PU A 1
O9' O -0.0436(6) 0.1940(5) 0.1481(5) 0.0296(10) Uani 0.494(7) 1 d P A 2
O10 O 0.1655(6) 0.2799(5) 0.1398(5) 0.0287(10) Uani 0.503(7) 1 d P A 1
O10' O 0.1462(6) 0.2422(6) 0.1009(5) 0.0287(10) Uani 0.497(7) 1 d P A 2
O11 O 0.2695(6) 0.1353(5) 0.0428(4) 0.0320(10) Uani 0.509(6) 1 d P A 1
O11' O 0.3371(6) 0.1534(5) 0.0496(4) 0.0320(10) Uani 0.491(6) 1 d PU A 2
O12 O 0.2817(19) -0.0653(6) -0.0063(5) 0.033(3) Uani 0.54(3) 1 d P A 1
O12' O 0.3476(18) -0.0536(6) 0.0000(5) 0.026(3) Uani 0.46(3) 1 d P A 2
O13 O -0.1604(4) -0.1610(3) 0.1003(3) 0.0685(15) Uani 1 1 d . . .
O14 O -0.1598(4) 0.0435(3) 0.1604(4) 0.0752(17) Uani 1 1 d . . .
O15 O -0.0125(4) -0.2778(6) 0.0259(3) 0.112(3) Uani 1 1 d . . .
O16 O 0.1879(5) -0.2270(6) -0.0118(3) 0.119(3) Uani 1 1 d . . .
O17 O 0.4085(3) -0.1732(3) 0.1259(3) 0.0468(9) Uani 1 1 d . A .
O18 O 0.3816(4) 0.0711(3) -0.0912(4) 0.0708(15) Uani 1 1 d . A .
O19 O 0.3896(4) 0.2285(3) 0.2132(3) 0.0542(11) Uani 1 1 d . A .
O20 O -0.0365(4) 0.3940(3) 0.1144(3) 0.0460(9) Uani 1 1 d . A .
O21 O 0.0220(5) 0.1290(4) 0.3150(2) 0.0648(13) Uani 1 1 d . A .
O22 O 0.0112(4) -0.2728(3) 0.1904(3) 0.0578(11) Uani 1 1 d . A .
O23 O -1.5167(6) 0.2976(7) -0.3074(5) 0.122(3) Uani 1 1 d . . .
O24 O -1.1334(5) 0.5349(4) 0.3157(5) 0.0911(19) Uani 1 1 d . . .
O25 O -0.2291(4) 0.3473(3) 0.4699(3) 0.0660(14) Uani 1 1 d . . .
N1 N -1.3273(6) 0.2691(5) -0.3173(4) 0.0756(17) Uani 1 1 d . . .
H1C H -1.2482 0.2843 -0.2936 0.091 Uiso 1 1 calc R . .
N2 N -1.3828(5) 0.4715(5) -0.0667(4) 0.0595(14) Uani 1 1 d . . .
N3 N -1.4050(5) 0.4107(6) 0.0837(4) 0.0661(16) Uani 1 1 d . . .
N4 N -1.0547(5) 0.3778(4) 0.3248(4) 0.0560(13) Uani 1 1 d . . .
H4A H -1.0579 0.3142 0.2976 0.067 Uiso 1 1 calc R . .
N5 N -0.3998(4) 0.3298(4) 0.3540(3) 0.0452(11) Uani 1 1 d . . .
H5B H -0.4481 0.2882 0.3088 0.054 Uiso 1 1 calc R . .
N6 N -0.1521(4) 0.0410(3) 0.4163(3) 0.0397(9) Uani 1 1 d . . .
C1 C -1.4340(11) 0.0007(15) -0.4739(8) 0.166(7) Uani 1 1 d . . .
H1A H -1.3828 0.0126 -0.5082 0.199 Uiso 1 1 calc R . .
H1B H -1.4195 -0.0684 -0.4601 0.199 Uiso 1 1 calc R . .
C2 C -1.3895(12) 0.0849(10) -0.3890(7) 0.117(4) Uani 1 1 d . . .
H2A H -1.4496 0.0815 -0.3595 0.140 Uiso 1 1 calc R . .
H2B H -1.3107 0.0667 -0.3529 0.140 Uiso 1 1 calc R . .
C3 C -1.3731(12) 0.1950(9) -0.3993(6) 0.107(3) Uani 1 1 d . . .
H3A H -1.3146 0.1989 -0.4300 0.128 Uiso 1 1 calc R . .
H3B H -1.4523 0.2151 -0.4332 0.128 Uiso 1 1 calc R . .
C4 C -1.4028(7) 0.3140(6) -0.2779(5) 0.0661(18) Uani 1 1 d . . .
C5 C -1.4217(5) 0.4126(5) -0.1444(5) 0.0563(15) Uani 1 1 d . . .
H5A H -1.5054 0.3877 -0.1679 0.068 Uiso 1 1 calc R . .
C6 C -1.3457(5) 0.3860(4) -0.1927(4) 0.0474(13) Uani 1 1 d . . .
C7 C -1.2226(5) 0.4275(5) -0.1592(4) 0.0508(14) Uani 1 1 d . . .
H7A H -1.1688 0.4139 -0.1907 0.061 Uiso 1 1 calc R . .
C8 C -1.1813(5) 0.4890(5) -0.0786(4) 0.0545(15) Uani 1 1 d . . .
H8A H -1.0987 0.5170 -0.0547 0.065 Uiso 1 1 calc R . .
C9 C -1.2623(6) 0.5092(6) -0.0329(5) 0.0597(16) Uani 1 1 d . . .
H9A H -1.2331 0.5496 0.0222 0.072 Uiso 1 1 calc R . .
C10 C -1.4432(7) 0.3091(8) 0.0697(5) 0.076(2) Uani 1 1 d . . .
H10A H -1.5122 0.2816 0.0221 0.091 Uiso 1 1 calc R . .
C11 C -1.3854(6) 0.2437(6) 0.1221(5) 0.0665(19) Uani 1 1 d . . .
H11A H -1.4152 0.1732 0.1101 0.080 Uiso 1 1 calc R . .
C12 C -1.2840(6) 0.2820(5) 0.1920(5) 0.0550(15) Uani 1 1 d . . .
H12A H -1.2429 0.2379 0.2277 0.066 Uiso 1 1 calc R . .
C13 C -1.3066(6) 0.4502(6) 0.1532(5) 0.0626(17) Uani 1 1 d . . .
H13A H -1.2802 0.5214 0.1642 0.075 Uiso 1 1 calc R . .
C14 C -1.2430(5) 0.3882(5) 0.2090(4) 0.0508(14) Uani 1 1 d . . .
C15 C -1.1387(6) 0.4400(5) 0.2874(5) 0.0553(15) Uani 1 1 d . . .
C16 C -0.9565(7) 0.4103(6) 0.4096(5) 0.072(2) Uani 1 1 d . . .
H16A H -0.9849 0.3850 0.4516 0.087 Uiso 1 1 calc R . .
H16B H -0.9475 0.4867 0.4247 0.087 Uiso 1 1 calc R . .
C17 C -0.8313(8) 0.3730(7) 0.4166(6) 0.081(2) Uani 1 1 d . . .
H17A H -0.7788 0.3888 0.4761 0.098 Uiso 1 1 calc R . .
H17B H -0.8400 0.2970 0.3971 0.098 Uiso 1 1 calc R . .
C18 C -0.7709(9) 0.4214(8) 0.3667(6) 0.089(3) Uani 1 1 d . . .
H18A H -0.7703 0.4975 0.3807 0.107 Uiso 1 1 calc R . .
H18B H -0.8158 0.3976 0.3061 0.107 Uiso 1 1 calc R . .
C19 C -0.6311(8) 0.3878(7) 0.3890(6) 0.084(2) Uani 1 1 d . . .
H19A H -0.5902 0.4021 0.4504 0.101 Uiso 1 1 calc R . .
H19B H -0.6316 0.3130 0.3672 0.101 Uiso 1 1 calc R . .
C20 C -0.5628(7) 0.4503(6) 0.3483(6) 0.077(2) Uani 1 1 d . . .
H20A H -0.5999 0.4289 0.2867 0.092 Uiso 1 1 calc R . .
H20B H -0.5756 0.5241 0.3636 0.092 Uiso 1 1 calc R . .
C21 C -0.4273(6) 0.4404(5) 0.3713(5) 0.0621(17) Uani 1 1 d . . .
H21A H -0.3933 0.4800 0.3389 0.075 Uiso 1 1 calc R . .
H21B H -0.3872 0.4705 0.4315 0.075 Uiso 1 1 calc R . .
C22 C -0.3041(5) 0.2913(4) 0.4048(3) 0.0404(11) Uani 1 1 d . . .
C23 C -0.1795(5) 0.1410(4) 0.4293(3) 0.0368(10) Uani 1 1 d . . .
H23A H -0.1230 0.1894 0.4735 0.044 Uiso 1 1 calc R . .
C24 C -0.2878(4) 0.1766(4) 0.3805(3) 0.0352(10) Uani 1 1 d . . .
C25 C -0.3708(5) 0.1033(4) 0.3145(3) 0.0424(11) Uani 1 1 d . . .
H25A H -0.4451 0.1236 0.2805 0.051 Uiso 1 1 calc R . .
C26 C -0.3424(5) 0.0004(4) 0.2998(3) 0.0448(12) Uani 1 1 d . . .
H26A H -0.3968 -0.0492 0.2554 0.054 Uiso 1 1 calc R . .
C27 C -0.2320(5) -0.0285(4) 0.3517(3) 0.0417(11) Uani 1 1 d . . .
H27A H -0.2129 -0.0981 0.3414 0.050 Uiso 1 1 calc R . .
O1W O -1.6544(7) 0.3096(5) -0.1157(6) 0.109(2) Uani 1 1 d . . .
O2W O -0.1022(4) -0.1257(3) 0.5097(3) 0.0552(11) Uani 1 1 d . . .
O3W O 0.0419(5) -0.1052(4) 0.3848(3) 0.0588(11) Uani 1 1 d . . .
O4W O -1.0828(6) 0.3147(4) -0.3714(3) 0.0890(19) Uani 1 1 d . . .
O5W O -0.2323(6) -0.2816(5) 0.3836(5) 0.096(2) Uani 1 1 d . . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
N6 Cu1 N6 179.998(1) 2_556 .
N6 Cu1 O2W 89.84(17) 2_556 .
N6 Cu1 O2W 90.16(17) . .
N6 Cu1 O2W 90.16(17) 2_556 2_556
N6 Cu1 O2W 89.84(17) . 2_556
O2W Cu1 O2W 180.0 . 2_556
N6 Cu1 O3W 88.62(17) 2_556 2_556
N6 Cu1 O3W 91.38(17) . 2_556
O2W Cu1 O3W 90.48(18) . 2_556
O2W Cu1 O3W 89.52(18) 2_556 2_556
N6 Cu1 O3W 91.39(17) 2_556 .
N6 Cu1 O3W 88.61(17) . .
O2W Cu1 O3W 89.52(18) . .
O2W Cu1 O3W 90.48(18) 2_556 .
O3W Cu1 O3W 179.997(1) 2_556 .
Cu2 Cu2 N3 103.8(7) 2_265 2_265
Cu2 Cu2 N2 86.8(6) 2_265 .
N3 Cu2 N2 92.3(3) 2_265 .
Cu2 Cu2 N2 76.0(6) 2_265 2_265
N3 Cu2 N2 91.8(3) 2_265 2_265
N2 Cu2 N2 162.82(10) . 2_265
Cu2 Cu2 N3 60.5(6) 2_265 .
N3 Cu2 N3 164.28(12) 2_265 .
N2 Cu2 N3 87.0(2) . .
N2 Cu2 N3 84.6(2) 2_265 .
O1 Si1 O1 180.0(3) . 2
O1 Si1 O2 67.1(3) . .
O1 Si1 O2 112.9(3) 2 .
O1 Si1 O2 112.9(3) . 2
O1 Si1 O2 67.1(3) 2 2
O2 Si1 O2 179.998(1) . 2
O1 Si1 O3 68.3(3) . 2
O1 Si1 O3 111.7(3) 2 2
O2 Si1 O3 109.5(3) . 2
O2 Si1 O3 70.5(3) 2 2
O1 Si1 O3 111.7(3) . .
O1 Si1 O3 68.3(3) 2 .
O2 Si1 O3 70.5(3) . .
O2 Si1 O3 109.5(3) 2 .
O3 Si1 O3 180.0 2 .
O1 Si1 O4 70.4(3) . .
O1 Si1 O4 109.6(3) 2 .
O2 Si1 O4 106.7(3) . .
O2 Si1 O4 73.3(3) 2 .
O3 Si1 O4 106.0(3) 2 .
O3 Si1 O4 74.0(3) . .
O1 Si1 O4 109.6(3) . 2
O1 Si1 O4 70.4(3) 2 2
O2 Si1 O4 73.3(3) . 2
O2 Si1 O4 106.7(3) 2 2
O3 Si1 O4 73.9(3) 2 2
O3 Si1 O4 106.1(3) . 2
O4 Si1 O4 180.0(4) . 2
O21 Mo1 O6' 114.6(3) . .
O21 Mo1 O5' 110.8(4) . .
O6' Mo1 O5' 87.1(4) . .
O21 Mo1 O5 94.6(3) . .
O6' Mo1 O5 99.5(4) . .
O5' Mo1 O5 17.2(3) . .
O21 Mo1 O6 92.3(3) . .
O6' Mo1 O6 22.5(2) . .
O5' Mo1 O6 98.3(4) . .
O5 Mo1 O6 105.6(4) . .
O21 Mo1 O14 97.2(3) . .
O6' Mo1 O14 146.9(3) . .
O5' Mo1 O14 89.9(4) . .
O5 Mo1 O14 86.0(3) . .
O6 Mo1 O14 164.4(3) . .
O21 Mo1 O9' 106.2(3) . .
O6' Mo1 O9' 88.2(3) . .
O5' Mo1 O9' 141.1(4) . .
O5 Mo1 O9' 152.4(4) . .
O6 Mo1 O9' 91.7(3) . .
O14 Mo1 O9' 73.8(2) . .
O21 Mo1 O9 87.0(3) . .
O6' Mo1 O9 89.5(3) . .
O5' Mo1 O9 161.6(4) . .
O5 Mo1 O9 169.1(4) . .
O6 Mo1 O9 85.1(3) . .
O14 Mo1 O9 83.1(2) . .
O9' Mo1 O9 20.6(2) . .
O21 Mo1 O2 156.5(2) . .
O6' Mo1 O2 55.1(3) . .
O5' Mo1 O2 90.7(4) . .
O5 Mo1 O2 107.6(3) . .
O6 Mo1 O2 74.6(2) . .
O14 Mo1 O2 92.1(2) . .
O9' Mo1 O2 55.9(2) . .
O9 Mo1 O2 72.7(2) . .
O21 Mo1 O1 156.9(2) . .
O6' Mo1 O1 87.2(3) . .
O5' Mo1 O1 60.4(4) . .
O5 Mo1 O1 73.3(3) . .
O6 Mo1 O1 109.7(3) . .
O14 Mo1 O1 63.0(2) . .
O9' Mo1 O1 80.8(2) . .
O9 Mo1 O1 101.3(2) . .
O2 Mo1 O1 43.93(18) . .
O22 Mo2 O15 102.0(3) . .
O22 Mo2 O13 101.9(2) . .
O15 Mo2 O13 98.1(2) . .
O22 Mo2 O5' 104.2(3) . .
O15 Mo2 O5' 150.6(4) . .
O13 Mo2 O5' 89.4(4) . .
O22 Mo2 O8' 109.2(3) . .
O15 Mo2 O8' 90.5(2) . .
O13 Mo2 O8' 145.3(3) . .
O5' Mo2 O8' 68.4(4) . .
O22 Mo2 O8 88.0(3) . .
O15 Mo2 O8 87.1(2) . .
O13 Mo2 O8 167.5(2) . .
O5' Mo2 O8 80.7(4) . .
O8' Mo2 O8 22.6(2) . .
O22 Mo2 O5 91.5(3) . .
O15 Mo2 O5 165.2(4) . .
O13 Mo2 O5 84.9(3) . .
O5' Mo2 O5 14.7(3) . .
O8' Mo2 O5 79.1(3) . .
O8 Mo2 O5 87.2(3) . .
O22 Mo2 O4 155.7(2) . .
O15 Mo2 O4 65.3(3) . .
O13 Mo2 O4 100.5(2) . .
O5' Mo2 O4 85.3(3) . .
O8' Mo2 O4 53.1(2) . .
O8 Mo2 O4 71.2(2) . .
O5 Mo2 O4 99.9(3) . .
O22 Mo2 O1 156.0(2) . .
O15 Mo2 O1 100.0(3) . .
O13 Mo2 O1 65.5(2) . .
O5' Mo2 O1 57.4(3) . .
O8' Mo2 O1 79.9(2) . .
O8 Mo2 O1 102.5(2) . .
O5 Mo2 O1 67.9(3) . .
O4 Mo2 O1 46.36(18) . .
O20 Mo3 O9' 112.3(3) . .
O20 Mo3 O16 102.7(3) . 2
O9' Mo3 O16 91.6(3) . 2
O20 Mo3 O10' 107.1(3) . .
O9' Mo3 O10' 91.8(3) . .
O16 Mo3 O10' 146.1(3) 2 .
O20 Mo3 O15 98.5(3) . 2
O9' Mo3 O15 148.3(3) . 2
O16 Mo3 O15 88.6(2) 2 2
O10' Mo3 O15 71.4(3) . 2
O20 Mo3 O9 93.5(2) . .
O9' Mo3 O9 20.2(3) . .
O16 Mo3 O9 103.4(3) 2 .
O10' Mo3 O9 90.7(3) . .
O15 Mo3 O9 160.7(3) 2 .
O20 Mo3 O10 91.1(2) . .
O9' Mo3 O10 87.9(3) . .
O16 Mo3 O10 165.3(3) 2 .
O10' Mo3 O10 19.4(2) . .
O15 Mo3 O10 84.1(2) 2 .
O9 Mo3 O10 80.6(3) . .
O20 Mo3 O4 155.02(19) . 2
O9' Mo3 O4 90.3(3) . 2
O16 Mo3 O4 64.6(3) 2 2
O10' Mo3 O4 81.6(2) . 2
O15 Mo3 O4 61.4(2) 2 2
O9 Mo3 O4 110.1(2) . 2
O10 Mo3 O4 100.7(2) . 2
O20 Mo3 O2 155.32(19) . .
O9' Mo3 O2 55.5(3) . .
O16 Mo3 O2 99.2(3) 2 .
O10' Mo3 O2 56.5(2) . .
O15 Mo3 O2 93.3(3) 2 .
O9 Mo3 O2 70.3(2) . .
O10 Mo3 O2 68.5(2) . .
O4 Mo3 O2 48.08(17) 2 .
O17 Mo4 O8' 114.4(3) . .
O17 Mo4 O7' 113.0(3) . .
O8' Mo4 O7' 81.3(3) . .
O17 Mo4 O12 108.2(6) . .
O8' Mo4 O12 135.6(6) . .
O7' Mo4 O12 93.4(3) . .
O17 Mo4 O7 94.7(3) . .
O8' Mo4 O7 99.4(3) . .
O7' Mo4 O7 21.6(3) . .
O12 Mo4 O7 88.7(4) . .
O17 Mo4 O8 92.3(2) . .
O8' Mo4 O8 23.2(3) . .
O7' Mo4 O8 96.4(3) . .
O12 Mo4 O8 151.7(6) . .
O7 Mo4 O8 109.5(3) . .
O17 Mo4 O16 98.4(3) . .
O8' Mo4 O16 89.4(3) . .
O7' Mo4 O16 148.4(3) . .
O12 Mo4 O16 72.4(4) . .
O7 Mo4 O16 159.6(3) . .
O8 Mo4 O16 85.6(2) . .
O17 Mo4 O12' 91.7(4) . .
O8' Mo4 O12' 153.7(5) . .
O7' Mo4 O12' 91.8(3) . .
O12 Mo4 O12' 18.8(3) . .
O7 Mo4 O12' 80.7(3) . .
O8 Mo4 O12' 168.7(4) . .
O16 Mo4 O12' 83.3(3) . .
O17 Mo4 O4 153.77(19) . .
O8' Mo4 O4 53.2(3) . .
O7' Mo4 O4 89.3(3) . .
O12 Mo4 O4 82.9(6) . .
O7 Mo4 O4 109.6(2) . .
O8 Mo4 O4 70.7(2) . .
O16 Mo4 O4 61.5(2) . .
O12' Mo4 O4 101.6(4) . .
O17 Mo4 O3 155.95(19) . .
O8' Mo4 O3 87.4(3) . .
O7' Mo4 O3 58.2(3) . .
O12 Mo4 O3 54.1(5) . .
O7 Mo4 O3 70.8(2) . .
O8 Mo4 O3 110.4(2) . .
O16 Mo4 O3 91.5(3) . .
O12' Mo4 O3 67.6(4) . .
O4 Mo4 O3 48.58(17) . .
O18 Mo5 O14 103.0(3) . 2
O18 Mo5 O12 113.9(7) . .
O14 Mo5 O12 92.6(4) 2 .
O18 Mo5 O12' 91.9(6) . .
O14 Mo5 O12' 104.2(4) 2 .
O12 Mo5 O12' 22.9(2) . .
O18 Mo5 O11 108.5(3) . .
O14 Mo5 O11 145.6(3) 2 .
O12 Mo5 O11 87.2(3) . .
O12' Mo5 O11 88.4(3) . .
O18 Mo5 O13 97.3(2) . 2
O14 Mo5 O13 88.02(17) 2 2
O12 Mo5 O13 147.7(6) . 2
O12' Mo5 O13 162.7(3) . 2
O11 Mo5 O13 74.8(2) . 2
O18 Mo5 O11' 87.8(3) . .
O14 Mo5 O11' 165.9(3) 2 .
O12 Mo5 O11' 91.4(3) . .
O12' Mo5 O11' 84.3(3) . .
O11 Mo5 O11' 21.2(2) . .
O13 Mo5 O11' 81.5(2) 2 .
O18 Mo5 O3 155.5(2) . .
O14 Mo5 O3 100.4(2) 2 .
O12 Mo5 O3 57.5(5) . .
O12' Mo5 O3 75.3(5) . .
O11 Mo5 O3 51.5(2) . .
O13 Mo5 O3 90.7(2) 2 .
O11' Mo5 O3 70.5(2) . .
O18 Mo5 O1 157.1(3) . 2
O14 Mo5 O1 65.2(2) 2 2
O12 Mo5 O1 87.1(7) . 2
O12' Mo5 O1 109.8(6) . 2
O11 Mo5 O1 80.5(2) . 2
O13 Mo5 O1 64.0(2) 2 2
O11' Mo5 O1 101.5(2) . 2
O3 Mo5 O1 44.63(18) . 2
O19 Mo6 O11 113.4(3) . .
O19 Mo6 O10' 113.0(3) . .
O11 Mo6 O10' 85.1(3) . .
O19 Mo6 O6' 108.0(3) . .
O11 Mo6 O6' 136.4(3) . .
O10' Mo6 O6' 91.4(3) . .
O19 Mo6 O10 93.9(3) . .
O11 Mo6 O10 102.7(3) . .
O10' Mo6 O10 21.8(2) . .
O6' Mo6 O10 87.4(3) . .
O19 Mo6 O11' 91.4(2) . .
O11 Mo6 O11' 22.1(2) . .
O10' Mo6 O11' 96.3(3) . .
O6' Mo6 O11' 154.4(3) . .
O10 Mo6 O11' 108.3(3) . .
O19 Mo6 O7' 104.6(3) . .
O11 Mo6 O7' 89.8(3) . .
O10' Mo6 O7' 140.9(3) . .
O6' Mo6 O7' 66.5(3) . .
O10 Mo6 O7' 151.5(3) . .
O11' Mo6 O7' 92.9(3) . .
O19 Mo6 O7 87.4(3) . .
O11 Mo6 O7 86.9(3) . .
O10' Mo6 O7 159.7(3) . .
O6' Mo6 O7 81.7(3) . .
O10 Mo6 O7 168.8(3) . .
O11' Mo6 O7 82.7(3) . .
O7' Mo6 O7 20.3(2) . .
O19 Mo6 O6 90.0(2) . .
O11 Mo6 O6 155.5(3) . .
O10' Mo6 O6 92.8(3) . .
O6' Mo6 O6 19.0(2) . .
O10 Mo6 O6 82.1(3) . .
O11' Mo6 O6 169.3(3) . .
O7' Mo6 O6 76.5(3) . .
O7 Mo6 O6 86.8(3) . .
O19 Mo6 O3 154.3(2) . .
O11 Mo6 O3 53.2(3) . .
O10' Mo6 O3 89.0(3) . .
O6' Mo6 O3 83.4(3) . .
O10 Mo6 O3 109.9(3) . .
O11' Mo6 O3 72.4(2) . .
O7' Mo6 O3 57.9(2) . .
O7 Mo6 O3 71.2(2) . .
O6 Mo6 O3 102.4(2) . .
O19 Mo6 O2 156.3(2) . .
O11 Mo6 O2 89.3(3) . .
O10' Mo6 O2 60.2(3) . .
O6' Mo6 O2 52.6(3) . .
O10 Mo6 O2 73.7(2) . .
O11' Mo6 O2 111.4(2) . .
O7' Mo6 O2 81.0(2) . .
O7 Mo6 O2 101.1(2) . .
O6 Mo6 O2 68.7(2) . .
O3 Mo6 O2 46.87(18) . .
Si1 O1 O2 57.8(2) . .
Si1 O1 O3 57.7(2) . 2
O2 O1 O3 96.6(3) . 2
Si1 O1 Mo1 123.5(3) . .
O2 O1 Mo1 65.9(2) . .
O3 O1 Mo1 138.5(3) 2 .
Si1 O1 Mo5 122.9(3) . 2
O2 O1 Mo5 127.3(3) . 2
O3 O1 Mo5 65.6(2) 2 2
Mo1 O1 Mo5 94.48(19) . 2
Si1 O1 Mo2 120.3(3) . .
O2 O1 Mo2 133.6(3) . .
O3 O1 Mo2 122.0(3) 2 .
Mo1 O1 Mo2 94.05(19) . .
Mo5 O1 Mo2 93.94(18) 2 .
Si1 O2 O1 55.1(2) . .
Si1 O2 Mo1 125.0(3) . .
O1 O2 Mo1 70.2(2) . .
Si1 O2 Mo6 120.4(3) . .
O1 O2 Mo6 139.8(3) . .
Mo1 O2 Mo6 97.00(19) . .
Si1 O2 Mo3 118.4(3) . .
O1 O2 Mo3 124.5(3) . .
Mo1 O2 Mo3 95.39(19) . .
Mo6 O2 Mo3 93.75(18) . .
Si1 O3 O1 54.0(2) . 2
Si1 O3 Mo5 123.4(3) . .
O1 O3 Mo5 69.8(2) 2 .
Si1 O3 Mo6 121.6(3) . .
O1 O3 Mo6 129.7(3) 2 .
Mo5 O3 Mo6 97.70(19) . .
Si1 O3 Mo4 117.9(3) . .
O1 O3 Mo4 133.6(3) 2 .
Mo5 O3 Mo4 94.89(19) . .
Mo6 O3 Mo4 94.72(19) . .
Si1 O4 Mo2 122.3(3) . .
Si1 O4 Mo3 119.7(3) . 2
Mo2 O4 Mo3 97.34(18) . 2
Si1 O4 Mo4 119.0(2) . .
Mo2 O4 Mo4 97.19(19) . .
Mo3 O4 Mo4 95.60(19) 2 .
Mo1 O5 Mo2 124.5(5) . .
Mo1 O5' Mo2 145.4(7) . .
Mo1 O6 Mo6 119.6(3) . .
Mo1 O6' Mo6 150.8(4) . .
Mo4 O7 Mo6 122.4(3) . .
Mo4 O7' Mo6 143.9(4) . .
Mo4 O8 Mo2 120.4(3) . .
Mo4 O8' Mo2 150.7(4) . .
Mo3 O9 Mo1 121.4(3) . .
Mo3 O9' Mo1 148.7(4) . .
Mo6 O10 Mo3 123.0(3) . .
Mo6 O10' Mo3 144.9(4) . .
Mo6 O11 Mo5 153.4(4) . .
Mo6 O11' Mo5 119.3(3) . .
Mo5 O12 Mo4 148.8(5) . .
Mo5 O12' Mo4 121.7(9) . .
Mo2 O13 Mo5 136.3(3) . 2
Mo5 O14 Mo1 136.9(3) 2 .
Mo2 O15 Mo3 135.7(4) . 2
Mo3 O16 Mo4 138.1(4) 2 .
C4 N1 C3 122.7(8) . .
C5 N2 C9 118.4(6) . .
C5 N2 Cu2 126.6(4) . .
C9 N2 Cu2 114.8(5) . .
C5 N2 Cu2 114.2(4) . 2_265
C9 N2 Cu2 126.8(5) . 2_265
Cu2 N2 Cu2 17.17(10) . 2_265
C10 N3 C13 118.2(7) . .
C10 N3 Cu2 110.5(6) . 2_265
C13 N3 Cu2 131.2(6) . 2_265
C10 N3 Cu2 126.2(6) . .
C13 N3 Cu2 115.5(5) . .
Cu2 N3 Cu2 15.72(12) 2_265 .
C15 N4 C16 124.9(6) . .
C22 N5 C21 122.9(5) . .
C23 N6 C27 118.5(4) . .
C23 N6 Cu1 118.3(3) . .
C27 N6 Cu1 123.1(4) . .
C1 C1 C2 115.5(15) 2_254 .
C3 C2 C1 115.2(12) . .
N1 C3 C2 112.3(9) . .
O23 C4 N1 123.0(8) . .
O23 C4 C6 118.8(7) . .
N1 C4 C6 118.2(6) . .
N2 C5 C6 123.8(6) . .
C5 C6 C7 117.8(6) . .
C5 C6 C4 117.2(6) . .
C7 C6 C4 125.0(6) . .
C8 C7 C6 118.7(6) . .
C7 C8 C9 119.9(6) . .
N2 C9 C8 121.2(7) . .
N3 C10 C11 122.8(7) . .
C12 C11 C10 119.8(7) . .
C11 C12 C14 118.8(7) . .
N3 C13 C14 122.1(7) . .
C13 C14 C12 118.3(7) . .
C13 C14 C15 118.5(6) . .
C12 C14 C15 123.1(6) . .
O24 C15 N4 122.7(7) . .
O24 C15 C14 120.4(6) . .
N4 C15 C14 116.9(6) . .
N4 C16 C17 116.2(7) . .
C18 C17 C16 112.6(8) . .
C17 C18 C19 108.0(8) . .
C20 C19 C18 108.1(7) . .
C21 C20 C19 115.9(7) . .
N5 C21 C20 111.6(6) . .
O25 C22 N5 122.0(5) . .
O25 C22 C24 120.5(5) . .
N5 C22 C24 117.6(4) . .
N6 C23 C24 123.5(4) . .
C23 C24 C25 117.4(5) . .
C23 C24 C22 116.3(4) . .
C25 C24 C22 126.3(4) . .
C26 C25 C24 119.5(5) . .
C25 C26 C27 119.3(5) . .
N6 C27 C26 121.8(5) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Cu1 N6 2.003(4) 2_556
Cu1 N6 2.003(4) .
Cu1 O2W 2.041(4) .
Cu1 O2W 2.041(4) 2_556
Cu1 O3W 2.346(4) 2_556
Cu1 O3W 2.346(4) .
Cu2 Cu2 0.607(3) 2_265
Cu2 N3 1.950(7) 2_265
Cu2 N2 1.995(6) .
Cu2 N2 2.053(6) 2_265
Cu2 N3 2.176(7) .
Si1 O1 1.573(5) .
Si1 O1 1.573(5) 2
Si1 O2 1.624(5) .
Si1 O2 1.624(5) 2
Si1 O3 1.642(5) 2
Si1 O3 1.642(5) .
Si1 O4 1.690(5) .
Si1 O4 1.690(5) 2
Mo1 O21 1.680(4) .
Mo1 O6' 1.744(7) .
Mo1 O5' 1.767(12) .
Mo1 O5 1.870(10) .
Mo1 O6 1.900(7) .
Mo1 O14 2.002(4) .
Mo1 O9' 2.009(7) .
Mo1 O9 2.055(7) .
Mo1 O2 2.325(5) .
Mo1 O1 2.395(5) .
Mo2 O22 1.654(4) .
Mo2 O15 1.805(5) .
Mo2 O13 1.810(4) .
Mo2 O5' 1.952(11) .
Mo2 O8' 1.969(7) .
Mo2 O8 2.083(7) .
Mo2 O5 2.140(10) .
Mo2 O4 2.318(5) .
Mo2 O1 2.457(5) .
Mo3 O20 1.650(3) .
Mo3 O9' 1.672(7) .
Mo3 O16 1.782(5) 2
Mo3 O10' 1.975(7) .
Mo3 O15 2.008(5) 2
Mo3 O9 2.011(7) .
Mo3 O10 2.128(7) .
Mo3 O4 2.385(5) 2
Mo3 O2 2.468(6) .
Mo4 O17 1.651(3) .
Mo4 O8' 1.691(8) .
Mo4 O7' 1.708(7) .
Mo4 O12 1.877(8) .
Mo4 O7 1.954(7) .
Mo4 O8 1.999(8) .
Mo4 O16 2.016(5) .
Mo4 O12' 2.183(13) .
Mo4 O4 2.404(5) .
Mo4 O3 2.467(5) .
Mo5 O18 1.645(4) .
Mo5 O14 1.790(4) 2
Mo5 O12 1.800(7) .
Mo5 O12' 1.868(8) .
Mo5 O11 1.965(7) .
Mo5 O13 2.023(4) 2
Mo5 O11' 2.110(7) .
Mo5 O3 2.339(5) .
Mo5 O1 2.411(5) 2
Mo6 O19 1.660(3) .
Mo6 O11 1.664(7) .
Mo6 O10' 1.743(7) .
Mo6 O6' 1.904(7) .
Mo6 O10 1.904(7) .
Mo6 O11' 1.981(7) .
Mo6 O7' 2.018(7) .
Mo6 O7 2.090(7) .
Mo6 O6 2.181(7) .
Mo6 O3 2.350(5) .
Mo6 O2 2.388(5) .
O1 O2 1.767(7) .
O1 O3 1.805(8) 2
O1 Mo5 2.411(5) 2
O3 O1 1.805(8) 2
O4 Mo3 2.385(5) 2
O13 Mo5 2.023(4) 2
O14 Mo5 1.790(4) 2
O15 Mo3 2.008(5) 2
O16 Mo3 1.782(5) 2
O23 C4 1.227(9) .
O24 C15 1.227(8) .
O25 C22 1.240(6) .
N1 C4 1.327(9) .
N1 C3 1.461(11) .
N2 C5 1.319(9) .
N2 C9 1.344(8) .
N2 Cu2 2.053(6) 2_265
N3 C10 1.331(11) .
N3 C13 1.341(10) .
N3 Cu2 1.950(7) 2_265
N4 C15 1.339(8) .
N4 C16 1.485(9) .
N5 C22 1.322(6) .
N5 C21 1.470(7) .
N6 C23 1.333(7) .
N6 C27 1.339(6) .
C1 C1 1.47(3) 2_254
C1 C2 1.560(15) .
C2 C3 1.483(15) .
C4 C6 1.495(10) .
C5 C6 1.375(8) .
C6 C7 1.383(8) .
C7 C8 1.371(10) .
C8 C9 1.378(9) .
C10 C11 1.364(12) .
C11 C12 1.361(10) .
C12 C14 1.391(9) .
C13 C14 1.387(9) .
C14 C15 1.496(10) .
C16 C17 1.488(11) .
C17 C18 1.457(12) .
C18 C19 1.600(12) .
C19 C20 1.500(12) .
C20 C21 1.476(10) .
C22 C24 1.499(7) .
C23 C24 1.386(6) .
C24 C25 1.389(7) .
C25 C26 1.374(8) .
C26 C27 1.385(7) .
